#------------------------------------------------------------------------------
#$Date: 2016-03-22 12:05:15 +0200 (Tue, 22 Mar 2016) $
#$Revision: 178933 $
#$URL: svn://www.crystallography.net/cod/cif/4/11/62/4116286.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4116286
loop_
_publ_author_name
'Cara C. Evans'
'Lisa Sukarto'
'Michael D. Ward'
_publ_section_title
;
 Sterically Controlled Architectural Reversion in Hydrogen-Bonded
 Crystalline Clathrates
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              320
_journal_page_last               325
_journal_paper_doi               10.1021/ja983122o
_journal_volume                  121
_journal_year                    1999
_chemical_compound_source        'C. Evans / Prof. M. Ward'
_chemical_formula_sum            'C14 H20 N8 O6 S2'
_chemical_formula_weight         460.50
_chemical_name_common
'guanidinium azobenzene-4,4'-disulfonate . nitrobenzene'
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL
_cell_angle_alpha                89.185(2)
_cell_angle_beta                 89.696(2)
_cell_angle_gamma                62.094(1)
_cell_formula_units_Z            1
_cell_length_a                   7.1781(3)
_cell_length_b                   7.3188(4)
_cell_length_c                   16.7531(7)
_cell_measurement_temperature    173(2)
_cell_volume                     777.70(6)
_computing_structure_refinement  'SHELXL-93 (Sheldrick, 1993)'
_computing_structure_solution    'SHELXS-86 (Sheldrick, 1990)'
_diffrn_ambient_temperature      173(2)
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0227
_diffrn_reflns_av_sigmaI/netI    0.0553
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            2660
_diffrn_reflns_theta_max         24.98
_diffrn_reflns_theta_min         1.22
_exptl_absorpt_coefficient_mu    0.204
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  0.663
_exptl_absorpt_correction_type   'SADABS (Shedrick, 1996)'
_exptl_crystal_colour            0.34
_exptl_crystal_density_diffrn    0.983
_exptl_crystal_description       Plate
_exptl_crystal_F_000             240
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.08
_refine_diff_density_max         0.670
_refine_diff_density_min         -0.509
_refine_diff_density_rms         0.068
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_all   1.122
_refine_ls_goodness_of_fit_obs   1.259
_refine_ls_matrix_type           full
_refine_ls_number_parameters     136
_refine_ls_number_reflns         2659
_refine_ls_number_restraints     12
_refine_ls_restrained_S_all      1.152
_refine_ls_restrained_S_obs      1.264
_refine_ls_R_factor_all          0.0841
_refine_ls_R_factor_obs          0.0673
_refine_ls_shift/esd_max         0.000
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.1212P)²+0.1350P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.2125
_refine_ls_wR_factor_obs         0.2000
_reflns_number_observed          1973
_reflns_number_total             2660
_reflns_observed_criterion       >2sigma(I)
_cod_data_source_file            ja983122o_2.cif
_cod_data_source_block           98099a
_cod_depositor_comments
;
The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc
w=1/[\s^2^(Fo^2^)+(0.1212P)^2^+0.1350P] where P=(Fo^2^+2Fc^2^)/3' was
changed to 'calc'. New tag '_refine_ls_weighting_details' was
created. The value of the new tag was set to
'w=1/[\s^2^(Fo^2^)+(0.1212P)^2^+0.1350P] where P=(Fo^2^+2Fc^2^)/3'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_database_code               4116286
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_thermal_displace_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
S1 S 0.19623(13) 0.39438(13) 0.36701(5) 0.0367(3) Uani 1 d .
O1 O 0.0893(4) 0.2779(4) 0.3950(2) 0.0492(7) Uani 1 d .
O2 O 0.0961(4) 0.6041(4) 0.39736(15) 0.0421(6) Uani 1 d .
O3 O 0.4224(4) 0.2876(4) 0.38150(15) 0.0404(6) Uani 1 d .
C1 C 0.1010(11) 0.4770(12) 0.1013(3) 0.126(3) Uani 1 d U
C2 C 0.2583(13) 0.4807(10) 0.1327(3) 0.104(2) Uani 1 d U
H2B H 0.3531(13) 0.5057(10) 0.1001(3) 0.125 Uiso 1 calc R
C3 C 0.2946(10) 0.4487(10) 0.2139(3) 0.091(2) Uani 1 d U
H3B H 0.4164(10) 0.4486(10) 0.2359(3) 0.109 Uiso 1 calc R
C4 C 0.1625(7) 0.4178(7) 0.2627(2) 0.0569(11) Uani 1 d U
C5 C -0.0011(12) 0.3984(22) 0.2281(4) 0.205(6) Uani 1 d U
H5A H -0.0871(12) 0.3579(22) 0.2592(4) 0.246 Uiso 1 calc R
C6 C -0.0375(13) 0.4391(25) 0.1468(5) 0.247(8) Uani 1 d U
H6A H -0.1579(13) 0.4409(25) 0.1227(5) 0.297 Uiso 1 calc R
N1 N 0.0775(10) 0.5033(12) 0.0141(3) 0.158(4) Uani 1 d .
C7 C -0.4643(5) 0.7347(5) 0.4209(2) 0.0358(8) Uani 1 d .
N2 N -0.3638(4) 0.5311(4) 0.4208(2) 0.0384(7) Uani 1 d .
H2C H -0.4353(4) 0.4610(4) 0.4201(2) 0.046 Uiso 1 calc R
H2D H -0.2251(4) 0.4653(4) 0.4213(2) 0.046 Uiso 1 calc R
N3 N -0.3561(5) 0.8410(5) 0.4227(2) 0.0447(8) Uani 1 d .
H3C H -0.2174(5) 0.7752(5) 0.4237(2) 0.054 Uiso 1 calc R
H3D H -0.4233(5) 0.9770(5) 0.4228(2) 0.054 Uiso 1 calc R
N4 N -0.6741(4) 0.8339(5) 0.4201(2) 0.0455(8) Uani 1 d .
H4A H -0.7453(4) 0.7634(5) 0.4195(2) 0.055 Uiso 1 calc R
H4B H -0.7416(4) 0.9699(5) 0.4202(2) 0.055 Uiso 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
O3 S1 O2 112.54(14) .
O3 S1 O1 113.21(14) .
O2 S1 O1 111.60(15) .
O3 S1 C4 106.5(2) .
O2 S1 C4 106.2(2) .
O1 S1 C4 106.2(2) .
C2 C1 C6 120.9(6) .
C2 C1 N1 117.7(8) .
C6 C1 N1 121.3(8) .
C1 C2 C3 120.7(7) .
C4 C3 C2 121.9(6) .
C3 C4 C5 117.6(5) .
C3 C4 S1 122.5(4) .
C5 C4 S1 119.8(4) .
C4 C5 C6 118.6(8) .
C1 C6 C5 119.8(8) .
N1 N1 C1 115.5(10) 2_565
N2 C7 N4 119.8(3) .
N2 C7 N3 120.0(3) .
N4 C7 N3 120.1(3) .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
S1 O3 1.455(2) .
S1 O2 1.455(2) .
S1 O1 1.461(3) .
S1 C4 1.761(4) .
C1 C2 1.260(9) .
C1 C6 1.375(13) .
C1 N1 1.472(7) .
C2 C3 1.384(7) .
C3 C4 1.343(7) .
C4 C5 1.378(8) .
C5 C6 1.390(11) .
N1 N1 1.233(15) 2_565
C7 N2 1.317(4) .
C7 N4 1.331(4) .
C7 N3 1.333(4) .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_4
C6 C1 C2 C3 -0.6(14) .
N1 C1 C2 C3 -177.4(6) .
C1 C2 C3 C4 -1.7(11) .
C2 C3 C4 C5 6.3(10) .
C2 C3 C4 S1 -175.6(5) .
O3 S1 C4 C3 -35.1(5) .
O2 S1 C4 C3 85.0(4) .
O1 S1 C4 C3 -156.1(4) .
O3 S1 C4 C5 142.9(7) .
O2 S1 C4 C5 -96.9(7) .
O1 S1 C4 C5 22.0(7) .
C3 C4 C5 C6 -8.6(15) .
S1 C4 C5 C6 173.3(9) .
C2 C1 C6 C5 -1.9(19) .
N1 C1 C6 C5 174.8(10) .
C4 C5 C6 C1 6.6(20) .
C2 C1 N1 N1 179.3(9) 2_565
C6 C1 N1 N1 2.6(15) 2_565
